Effect of Chlorhexidine Application Protocol on Durability of
Marginal Seal of Class V Restorations
Anna Saffarpour 1, Aida Saffarpour 2,Mohammad Javad Kharazifard 3, Atoussa Entezami Rad 4
1 Assistant Professor, Department of Periodontics, Dental Faculty, Tehran University of Medical Sciences (International Campus) , Tehran, Iran 2 Assistant Professor, Department of Operative Dentistry, Dental Faculty, Tehran University of Medical Sciences (International Campus),
3 Epidemiologist, Dental Research Center, Dentistry Research Institute, Tehran University of Medical Sciences, Tehran, Iran 4 Dentist, Tehran, Iran
Objectives: This study aimed to evaluate the effect of chlorhexidine (CHX) application protocol on durability of marginal seal of class V composite restorations.
Materials and Methods: Class V cavities (4×2×1.5mm) were prepared in the buccal surfaces of 160 human third molars. The teeth were randomly divided into five groups (n=32) of (G1) CHX+rinse+etching, (G2) CHX+etching, (G3) etching+CHX+rinse, (G4) etching+ CHX, and (G5) etching alone as the control group. Adper Single Bond 2 was applied as an etch and rinse (E & R) bonding system. Cavities were filled with Z350 composite. Half of the teeth in each group were stored in distilled water for 24 hours and the other half were thermocycled (10,000 cycles, 5-55˚C). For dye penetration test, the teeth were sectioned buccolingually and assessed at the enamel and dentin margins under a stereomicroscope at ×20 magnification. The Kruskal-Wallis, Dunn and Mann-Whitney tests were used for statistical analyses.
Results: There was no significant difference in immediate microleakage among the groups at the enamel and dentin margins (P= 0.894). After thermocycling, there was significantly less microleakage in G4 than the control group at dentin margin. There were significant differences in microleakage between G4 and G1(P=0.002), G4 and G2 (P=0.001) and G4 and G5 (P= 0.001) at dentin margin.
Conclusions: Application of CHX after etching without rinsing is effective to decrease microleakage. However, it has no effect if applied before etching in use of this particular type of E & R adhesive after thermocycling.
Keywords: Dental Leakage; Chlorhexidine; Composite Resins
Journal of Dentistry, Tehran University of Medical Sciences, Tehran, Iran (2016; Vol. 13, No. 4)
A. Saffarpour, Department of Operative Dentistry, Dental Faculty, Tehran University of Medical Sciences (International Campus), Tehran, Iran
Received: 24 February 2016 Accepted: 28 May 2016
Microleakage is defined as penetration of fluids, bacteria, molecules and ions through the interface of restorative material and cavity wall, which is not clinically detectable . This phenomenon can cause marginal staining of
restorations, postoperative tooth
hyper-sensitivity, secondary caries, pulpal pathology, or complete loss of restoration . In spite of chemical and technical advances in adhesive systems, obtaining an adequate gingival seal in dentin is still a major problem. In order to evaluate the marginal seal and the performance of hybrid layer, the specimens are submitted to leakage tests. Thus, degree of dye penetration through the bonding interface can reveal the
adaptation of restorative material to cavity walls .
dentin etching may partially denature the MMPs. On the other hand, mild acids such as those incorporated in simplified E & R systems can activate MMPs .
Even if a perfect seal is achieved with a restoration, residual bacteria can still proliferate and cause pulpal irritation and deteriorate the problems related to microleakage overtime . To solve this problem, cavity disinfectant solutions have been introduced . Some studies have recommended the application of chlorhexidine (CHX) before bonding procedures because of its antimicrobial effects [11,12]. Pashley et al,  reported that application of CHX to acid-etched dentin may be a preventive strategy against degradation of collagen fibrils. As a result, in addition to its known disinfectant effect, CHX acts as a MMP inhibitor . Also, CHX can prevent or reduce the degradation of exposed collagen fibrils present in imperfect hybrid layers. Therefore, the stability of the hybrid layer is preserved over time . Moreover, CHX application can be a more practical method than other techniques for rehydrating the dried demineralized dentin in order to preserve the necessitous humidity to preserve expansion of collagen network . In addition, there is controversy in the literature about the effect of CHX on bonding strength or microleakage of restorations [6,7,15-17]. In fact, to our knowledge, little information exists about sealing ability and durability of E & R adhesives in combination with CHX. Thus, the present in-vitro study aimed to assess the marginal sealing ability of CHX with different application protocols in class V restorations. Our hypotheses were: 1. CHX would have no adverse effect on microleakage of class V cavities. 2. CHX application methods prior to bonding procedure (before or after acid etching) would not affect microleakage after thermocycling.
MATERIALS AND METHODS
One hundred and sixty caries-free, intact human
third molars were used in this study. Tissue residues and calculus were removed and the crowns were cleaned with a rotary dental prophylaxis instrument. The teeth were stored in 1% chloramine T solution at 4°C for one week before use. Standard class V cavities (4mm long, 2mm high,1.5mm deep) were prepared in the buccal surface of each tooth, with occlusal margins 1mm above the cementoenamel junction and gingival margins 1mm below it, using a straight diamond bur (78 #8, d2; Teeskavan, Tehran, Iran) in a high speed handpiece under constant air-water spray. After five preparations, the diamond bur was replaced with a new one. The specimens were randomly assigned to five groups of 32 teeth each, corresponding to each application protocol.
Group 1 (CHX+rinse+etching): In this group, 1mL of 2% CHX solution (Consepsis, Ultradent Product Inc., South Jordan, UT, USA) was applied for 35 seconds in cavities, rinsed with water spray for 20 seconds, etched with 37% phosphoric acid (3M ESPE, St. Paul, MN, USA) for 15 seconds, rinsed with water spray for 15 seconds and gently air dried for 10 seconds. Two layers of Adper Single Bond 2 adhesive (3M ESPE, St. Paul, MN, USA) were then applied.
Group 2 (CHX+etching): Consepsis CHX solution was applied before acid etching as in group 1, with an exception that it was just air dried with no rinse off.
Group 3 (etching+CHX+rinse): Consepsis CHX solution was applied after acid etching for 35 seconds, rinsed for 20 seconds and carefully blot-dried with a sterile microbrush. Acid etching and bonding procedures were performed as previously described.
Group 4 (etching+CHX): Consepsis CHX solution was applied after acid etching as in group 3, with an exception that it was just air-dried without rinsing.
For all the cavities, the bonding and filling protocols were performed using Adper Single Bond 2 (3M ESPE, St Paul, MN, USA) two-step E & R adhesive and Filtek Z350 (3M ESPE, St. Paul, MN, USA) nanohybrid composite in two oblique increments. Curing was performed using Valo light curing unit (Ultradent Product Inc., South Jordan, UT, USA) with 1000mW/cm2 light intensity for 20 seconds. All the materials were used according to the manufacturers’ instructions.
Table 1 shows the composition of materials used in the present study and manufacturers’
instructions. Following the pretreatment
procedure in each group and filling of cavities, the restorations were finished using carbide finishing burs (#448L,012; Ultradent Product Inc., South Jordan, UT, USA) and Kerr discs (Opti Disc; Kerr, Orange, CA, USA).
Half of the specimens in each group were randomly selected and stored in distilled water at 37°C for 24 hours until microleakage testing. The remaining half were thermocycled for 10,000 cycles between 5°C to 55°C, with a dwell time of 30 seconds and transfer time of 15 seconds. After storage or thermocycling, the specimens were blot-dried and the root apices were sealed with modeling wax. The specimens were immersed in 2% basic fuchsine dye at 37°C for 24 hours separately.
After dye storage, the teeth were rinsed with water in order to remove excess dye. The teeth were then sectioned buccolingually through the center of restorations with a diamond disc (Leitz1600, Leica Instruments GmbH, Koln, Germany) under water. Dye penetration was assessed using a stereomicroscope (SMZ800, Nikon, Tokyo, Japan) at ×20 magnification. Both gingival (dentin) and occlusal (enamel) margins were evaluated by two blind examiners using the following scale:
0: No leakage;
1: Leakage up to one-third of depth of the cavity wall;
2: Leakage up to two-thirds of depth of the cavity wall, not including the axial wall; and
3: Leakage along the axial wall .
Statistical analysis: The Kruskal-Wallis test,
Dunn test and Mann-Whitney test were used for statistical analyses. The level of statistical significance was set at P<0.05.
The amount of dye penetration and the microleakage scores of the enamel and dentin margins are presented in Table 2. The Kruskal-Wallis test showed that there was no significant difference in microleakage at the enamel (P=0.834) or dentin (P=0.894) margins among the five immediate groups.
Table 1: Materials’ brand names, composition and manufacturers’ instructions
brand name Composition Manufacturer Method of application
Etchant 37% Phosphoric acid
3M ESPE Dental Products, St. Paul, MN, USA
G1,3&5: 15 sec. etching+15 sec. rinsing G2&4: 15 sec. etching without rinsing
Adper Single Bond 2
Ethyl alcohol, Bis-GMA,HEMA, glycerol,3-dimethacrylate, acrylic acid copolymer, itaconic acid, diurethane dimethacrylate, water, colloidal filler
3M ESPE Dental Products,
St. Paul, MN, USA G 1-5: Two layers applied & cured
Filtek Z-350 Bis-GMA, UDMA, TEGDMA,
ethyl methacrylate, inorganic fillers
3M ESPE Dental Products, St. Paul, MN, USA
G 1-5: Two oblique increments applied in cavity and cured
Consepsis 2% 2% Chlorhexidine Ultradent Products, South Jordan, UT, USA
However, among the five thermocycled groups, a significant difference existed in microleakage at the dentin margin (P<0.001) while the difference in microleakage at the enamel margin
was no significant (P=0.859). Pairwise
comparisons by Dunn test (Table 3) revealed that in thermocycled groups, a significant difference existed between G1 (CHX+rinse+etching) and G4 (etching+CHX) (P=0.002), G2 (CHX+ etching) and G4 (P=0.001) and G5 (control) and G4 (P<0.001). Mann-Whitney U test was used to compare microleakage in immediate and thermocycled groups. In G1 (CHX+rinse+
etching) (P<0.001), G2 (CHX+etching)
(P<0.001), G3 (etching+CHX+rinse) (P=0.019) and G5 (control)(P<0.001) greater microleakage was observed at the dentin margins of thermocycled specimens compared to non-thermocycled samples.
The present in-vitro study assessed the marginal sealing ability of CHX with different application protocols in class V composite restorations. Based on the results of the present study, various application protocols of 2% CHX did not show any adverse effect on immediate sealing ability of Adper Single Bond 2 total etch adhesive system.
Thus, the first hypothesis was supported. This result was supported by other studies [7,9]. The most probable explanation for this finding is that application of CHX before or after etching can improve the tooth surface energy and wettability of adhesive . After 10,000 thermal cycles, the groups, which received CHX application showed greater microleakage compared to the immediate groups. Thus, the second hypothesis was not supported.
*Statistically significant (P<0.05)
Table 2: Microleakage scores of the enamel and dentin margins with and without thermocycling
Immediate N(%) Thermocycled N(%)
margin 0 1 2 3
margin 0 1 2 3
G 1 E 14(87.5) 2(12.5) 0 0 E 12(75.0) 4(25.0) 0 0
D 3(18.8) 11(68.8) 2(12.5) 0 D 0 2(12.5) 12(75.0) 2(12.5)
G2 E 14(87.5) 2(12.5) 0 0 E 11(68.8) 5(31.3) 0 0
D 5(31.3) 8(50.0) 3(18.8) 0 D 0 2(12.5) 11(68.8) 3(18.8)
G3 E 15(93.8) 1(6.3) 0 0 E 13(81.3) 3(18.8) 0 0
D 5(31.3) 9(56.3) 2(12.5) 0 D 1(6.3) 8(50.0) 6(37.5) 1(6.3)
G4 E 13(81.3) 3(18.8) 0 0 E 13(81.3) 3(18.8) 0 0
D 5(31.3) 9(56.3) 2(12.5) 0 D 3(18.8) 10(62.5) 3(18.8) 0
E 13(81.3) 3(18.8) 0 0 E 11(68.8) 5(31.3) 0 0
D 3(18.8) 10(62.5) 3(18.8) 0 D 0 3(18.8) 7(43.8) 6(37.5)
Table 3: Pairwise comparisons of the groups after thermocycling
G1 (CHX+rinse+etching) - P>0.999 P=0.294 P=0.002* P>0.999
G2 (CHX+etching) - - P=0.169 P=0.001* P>0.999
G3 (etching+CHX+rinse) - - - P>0.999 P=0.059
G4 (etching+CHX) - - - - P<0.001*
Although the reduction in microleakage in CHX groups was greater than that in the control group, the results showed that CHX was unable to perfectly prevent microleakage in long-term. According the results of this study, after thermocycling there were significant differences between G1 (CHX+rinse+etching) and G4 (etching+CHX), G2 (CHX+rinse+etching) and G4, and G5 (control) and G4. In this study, Consepsis CHX solution was applied for its antibacterial activity to eliminate residual bacteria, as reported in other studies [12,19]. The least microleakage score was noted in G4 (etching+CHX) in our study. The other important issue associated with application of CHX is its inhibitory effect on MMPs, which are responsible for bond failure in long-term . With regard to long term bond failure of E & R adhesives, two hypotheses have been suggested: First, application of low pH phosphoric acid for dentin etching can partially denature MMPs. Mild acids like those incorporated in E & R adhesives have the ability to activate new MMPs . Furthermore, naked collagen fibrils, which are present at the bottom of the hybrid layer as a result of incomplete resin infiltration, are susceptible to MMP degradation . Moreover, most simplified adhesives act as a semi-permeable membrane after curing. Breschi et al,  assumed that water can pervade into the adhesive interface and subsequently activate MMPs, leading to degradation of infiltrated collagen fibrils. It seems that collagenases need water to be activated for hydrolysis . Due to water sorption mechanism, some of the hydrophilic monomers are removed from the hybrid layer; thus, the amount of exposed collagen fibrils will increase. This, in turn, will lead to enzymatic cleavage . In case of E & R adhesives, decreased infiltration of resin may result in formation of unprotected collagen fibrils at the bottom of hybrid layer, which are also susceptible to hydrolytic degradation [21,22]. A scanning electron microscopic study reported
adhesion . According to the results of this study, after thermocycling, microleakage score was high in G3 (etching+CHX+rinse). On the contrary, G4 (etching+CHX) showed the same microleakage score as that of groups before thermocycling. These results were in agreement with those of Carrilho et al,  who showed that CHX acts as a MMPs inhibitor when applied prior to bonding without rinsing. Thus, it preserves dentin bond strength . In fact, the naked collagen fibrils are accessible to CHX in the mentioned protocol. Consequently, they are sealed with adhesive resins. This procedure could preserve them in a better way. Contrary to the current study results, some studies have reported interference of CHX with bonding procedure and consequent reduction in bond strength or increase in microleakage particularly in use of self-etching adhesive systems [17,27]. It seems that cavity disinfectants applied to dentin surfaces are resistant to acid conditioning. Moreover, this acid-resistant layer might inhibit the weak acidic primers to effectively demineralize dentin and prevent the hydrophilic resin to impregnate the dentinal surface . Considering the antimicrobial activity of CHX , its chelating action and bond to several proteins  and no interference with the bonding process, it would be beneficial to preserve the collagen fibrils in hybrid layer by application of CHX without rinsing after acid etching of dentin in order to prevent degradation over time. In addition, since CHX has high water content, it can rehydrate the dried and demineralized dentin, and decrease the technical sensitivity of total etch adhesives. Nevertheless, more in vitro and in vivo studies are required to assess the effects of various concentrations of CHX on marginal seal and bond strength over time.
Within the limitations of this study, the results showed that application of CHX after etching had
no adverse effect on microleakage scores in all groups. Thermocycling did not have any effect on microleakage of CHX groups.
1- Fabianelli A, Pollington S, Davidson CL, Cagidiaco MC, Gorraci C. The relevance of micro-leakage studies. Int Dent SA. 2007;9(3):64-74. 2- Guzman-Ruiz S, Armstrong SR, Cobb DS, Vargas MA. Association between microtensile bond strength and leakage in the indirect resin composite/dentin adhesively bonded joint. J Dent. 2001 Feb;29(2):145-53.
3- Ito S, Hashimoto M, Wadgaonkar B, Svizero N, Carvalho RM, Yiu C, et al. Effects of resin hydrophilicity on water sorption and changes in
modulus of elasticity. Biomaterials. 2005
4- Boruziniat A, Babazadeh M, Gifani M. Effect of chlorhexidine application on bond durability of a filled-adhesive system. J Dent Mat Tech 2013 Mar;2(1):6-10.
5- Pashley DH, Tay FR, Tiu C, Hashimoto M, Breschi L, Carvalho RM. Collagen degradation by host-derived during aging. J Dent Res. 2004 Mar;83(3): 216-21.
6- Breschi L, Cammeli F, Visiniti E, Mazzoni A, Vita F, Carrilho M, et al. Influence of chlorhexidine concentration on the durability of etch-and-rinse dentin bonds: a 12-month in vitro study. J Adhes Dent. 2009 Jun;11(3):191-8.
7- Chang YE, Shin DH. Effect of chlorhexidine application methods on microtensile bond strength to dentin in class I cavities. Oper Dent. 2010 Nov-Dec;35(6):618-23.
8- Mazzoni A, Pashley DH, Nishitani Y, Brechin L, Mannello F, Tjaderhane L, et al. Reactivation of inactivated endogenous proteolytic activities in phosphoric acid-etched dentin by etch-and-rinse adhesives. Biomaterials. 2006 Sep;27(25):4470-6. 9- Shafie F, Doozandeh M, Alavi A. Effect of resin coating and chlorhexidine on microleakage of two resin cements after storage. J Dent (Tehran). 2010 Winter;7(1):31-40.
Willershausen B. Comparison of the efficacy of chemomechanical caries removal(Carisolv) with that of conventional excavation in reducing the cariogenic flora. Int J Paediatr Dent. 2004 May;14(3):182-91. 11- Fardal O, Turnbull RS. A review of the literature on use of chlorhexidine in dentistry. J Am Dent Assoc. 1986 Jun;112(6):863-9.
12- Sobral MA, Garone-Netto N, Luz MA, Santos AP. Prevention of postoperative sensitivity: a preliminary clinical trial. J Oral Rehabil. 2005 Sep;32 (9):661-8.
13- Hebling J, Pashley DH, Tjaderhane L, Tay FR. Chlorhexidine arrests subclinical degradation of dentin hybrid layers in vivo. J Dent Res. 2005 Aug; 84(8):741-6.
14- Soares CJ, Pereira CA, Pereira JC, Santana FR, do Prado CJ. Effect of chlorhexidine application on microtensile bond strength to dentin. Oper Dent. 2008 Mar-Apr;33(2):183-8.
15- Carrilho MR, Carvalho RM, de Goes MF, di Hipolito V, Geraldeli S, Tay FR, et al. Chlorhexidine preserves dentin bond in vitro. J Dent Res. 2007 Jan;86(1):90-4.
16- Elkassas DW, Fawzi EM, El Zohairy A. The effect of cavity disinfectants on the micro-shear bond strength of dentin adhesives. Eur J Dent. 2014 Apr;8(2):184-90.
17-Sharma V, Nainan MT, Shivanna V. The effect of cavity disinfectants on the sealing ability of dentin bonding system: An in vitro study. J Conserv Dent. 2009 Jul;12(3):109-13.
18- de Castro FL, de Andrade MF, Durate Junior SL, Vaz LG, Ahid FJ. Effect of 2% chlorhexidine on microtensile bond strength of composite to dentin. J Adhes Dent. 2003 Summer;5(2):129-38.
19- Darabi F, Eftekhari M. Effect of chlorhexidine on microleakage of composite restorations. J Dent (Tehran). 2009 Jan;6(1):16-22.
20- De Munck J, Van Meerbeek B, Yoshida Y, Inoue S, Vargas M, Suzuki K, et al. Four-year water degradation of total-etch adhesives bonded to dentin. J Dent Res. 2003 Feb;82(2):136-40.
21- Hashimoto M, Ohno H, Sano H, Tay FR, Kaga M, Kudou Y, et al. Micromorphological changes in resin-dentin bonds after 1 year of water storage. J Biomed Mater Res. 2002;63(3): 306-11.
22- Hashimoto M, Ohno H, Kaga M, Endo K, Sano H, Oguchi H. In vivo degradation of resin-dentin bonds in humans over 1 to 3 years. J Dent Res. 2000 Jun;79(6):1385-91.
23- Visse R, Nagase H. Matrix metalloproteinases and tissue inhibitors of metalloproteinases: Structure, function and biochemistry. Circ Res. 2003 May;92 (8):827-39.
24- Malacrane J, Carvalho RM, de Goes MF, Svizero
N, Pashley DH, Tay FR, et al. Water
sorption/solubility of dentinal adhesives resins. Dent Mater. 2006 Oct;22(10):973-80.
25- Predigao J, Denehy GE, Swift EJ Jr. Effects of chlorhexidine on dentin surfaces and shear bond strengths. Am J Dent. 1994 Apr;7(2):81-4.
26- Say EC, Koray F, Tarim B, Soyman M, Gulmez T. In vitro effect of cavity disinfectants on bond strength of dentin bonding systems. Quintessence Int. 2004 Jan;35(1):56-60.